|Year : 2023 | Volume
| Issue : 1 | Page : 3
Evaluation of surface-modified orthodontic wires by different concentration and dipping duration of titanium oxide (TiO2) nanoparticles
TP Chaturvedi1, P Indumathi1, Vipul Kumar Sharma1, Ashish Agrawal1, Deepak Singh1, Chandan Upadhyay2
1 Orthodontic Unit, Faculty of Dental Sciences, Institute of Medical Sciences, Banaras Hindu University, Varanasi, Uttar Pradesh, India
2 School of Material Science and Technology, IIT (BHU), Varanasi, Uttar Pradesh, India
|Date of Submission||04-May-2022|
|Date of Decision||15-Jul-2022|
|Date of Acceptance||04-Aug-2022|
|Date of Web Publication||18-Mar-2023|
Vipul Kumar Sharma
Orthodontic Unit, Faculty of Dental Sciences, Institute of Medical Sciences, Banaras Hindu University, Varanasi - 221005, Uttar Pradesh
Source of Support: None, Conflict of Interest: None
OBJECTIVE: To evaluate in-vitro surface characteristics and frictional properties of orthodontic stainless steel and beta-titanium archwires after surface modification with different concentrations and coating time of titanium oxide (TiO2) nanoparticles by Sol-gel dip coating method.
MATERIALS AND METHODS: The experiment was carried out with 4 different concentrations (1:2, 1:4, 1:6, and 1:8) and three different dipping durations (24 hours, 48 hours, and 72 hours) over ten main test groups of SS and TMA archwires with uncoated wires acting as control in both dry and wet conditions. Phase analysis and surface characterization of TiO2 was analyzed by X-ray Diffractometry, surface evaluation with the help of scanning electron microscopy (SEM), and frictional characteristics were evaluated.
RESULTS: Among all the concentrations 1:6 ratio with 48 hours of dipping duration showed better surface characteristics. A statistically significant difference in frictional coefficient was observed in both SS and TMA wires than their respective controls (p = 0.001). Intragroup comparison among SS and TMA groups showed that groups with 1:6 ratio and 48 hours dipping duration had least frictional coefficient in both dry and wet conditions (p = 0.001). Intergroup comparison between SS and TMA showed that SS group had significantly reduced friction than TMA (p = 0.001) except in few groups.
CONCLUSION: TiO2 nanoparticle with a concentration ratio of 1:6 and 48 hours dipping duration is recommended for surface modification of orthodontic archwires.
Keywords: Coating, friction, nanoparticles, orthodontic wires, surface modification
|How to cite this article:|
Chaturvedi T P, Indumathi P, Sharma VK, Agrawal A, Singh D, Upadhyay C. Evaluation of surface-modified orthodontic wires by different concentration and dipping duration of titanium oxide (TiO2) nanoparticles. J Orthodont Sci 2023;12:3
|How to cite this URL:|
Chaturvedi T P, Indumathi P, Sharma VK, Agrawal A, Singh D, Upadhyay C. Evaluation of surface-modified orthodontic wires by different concentration and dipping duration of titanium oxide (TiO2) nanoparticles. J Orthodont Sci [serial online] 2023 [cited 2023 Mar 25];12:3. Available from: https://www.jorthodsci.org/text.asp?2023/12/1/3/371964
| Introduction|| |
Selection of an appropriate archwire requires thorough knowledge of the archwire's biomechanical and clinical applications. Moreover, among the properties of an alloy that alter the behavior of the archwire, surface characteristics play a crucial role. Surface topography of an archwire can affect its mechanical characteristics, corrosion behavior, friction, aesthetic appearance, and biocompatibility. The retarding frictional force develops due to the surface roughness of the archwire. Nanoengineering-based surface modification can be used to reduce the surface roughness of orthodontic wires. Studies have demonstrated a reduction in the surface roughness and friction on the coating of archwires such as diamond-like carbon, Teflon, and fullerene-like nanoparticles. Anuradha et al. reported that sputter coating with titanium on archwires reduces surface roughness. Furthermore, other studies have focused on bacterial adhesion based on the photocatalytic activity of TiO2., Liu et al. reported that the corrosion resistance of the composite archwire might be substantially upgraded after coating with the TiO2 nanocrystal thin film. Owing to its beneficial characteristics such as biological stability, antibacterial property, and high frictional resistance, titanium dioxide (TiO2) has been receiving considerable attention in recent years compared with other nanoparticles used for the surface modification of orthodontic archwires. To the best of our knowledge, rarely any study has evaluated the surface roughness and frictional resistance of surface-modified orthodontic wires by using different concentrations of TiO2 nanoparticles at different coating times.
| Materials and Methods|| |
This study was conducted at the Department of Orthodontics in collaboration with the School of Materials Science and Technology. The study was approved by the institutional ethical committee (DEAN/2019/EC/1155). Preformed straight-length rectangular stainless steel (SS) and beta-titanium (TMA) archwires (Ormco. Corp) were used in this study. The study was performed using 260 specimens of orthodontic wires, with each being 65 mm in length. The specimens were divided into 10 main test groups. The groups containing uncoated SS and uncoated beta-titanium wires acted as the control group for their respective experimental group. Each group except the control group (Group 1-ST and Group 2-TT) was divided into three sub-groups based on the dipping duration of the respective colloidal solution of TiO2 [Table 1]. The nanocrystalline anatase phase of TiO2 with different ratios (1:2, 1:4, 1:6, and 1:8) was prepared [Table 2]. The sol-gel method was used for coating at room temperature without any heat treatment. Before deposition, the bare SS and TMA wires were cleaned in dilute H2SO4 and absolute ethanol solution. The substrates were immersed in the coating solutions of different concentrations and withdrawn at a series of three different immersion timings of 24 hours, 48 hours, and 72 hours. After withdrawal from the solution, the wires were dried in an oven at 60°C for 5 min. The formation and phase analyzes of obtained TiO2 were performed using the Rigaku X-ray diffractometer (XRD). Surface morphology of the uncoated and coated SS and TMA wires was examined through scanning electron microscopy (SEM; Nova Nano SEM 450). Tidy's protocol was adopted to determine frictional characteristics. All the tests were conducted in both dry and wet (artificial saliva) conditions by using an Instron universal testing machine (Instron corp., model number- 3379). The bracket and wire were replaced after sliding each sample to ensure the similarity of conditions for all the samples.
| Results|| |
[Figure 1] shows the diffraction pattern of 1:6 TiO2 nanoparticles coated on SS and TMA wires. The diffraction patterns obtained were similar for all the four different colloidal solution concentration. The very first observation of the diffraction pattern is broad diffraction peaks indicating the TiO2 crystallites to be in a nanometre range. Results of phase analysis, showed that there was 83% of anatase phase and 17% of rutile phase of TiO2. Further, the particle size of the anatase phase in all concentrations has a similar size of 7 nm. In the [Figure 2]a, we can observe the rough surface morphology of Group 1-ST, that is, uncoated SS wire. The uncoated SS archwire surface is full of pits and wedges adding to a rough surface. In [Figure 2]b and [Figure 2]c, the microphotographs of Group 2-ST24, Group 2-ST48, and Group 2-ST72 which were coated with the solution ratio 1:2, smooth surface morphology without any pits and voids are evident. In Group 2-ST72, slight irregularity was observed [Figure 2]d. In Group 3-ST72', more irregularity was observed as compared with Group 2-ST24' and Group 2-ST48' [Figure 2]e. Group 2-ST48 showed relatively soother surface when compared with other groups. In [Figure 2]f, we can observe a smooth surface morphology of Group 4-ST48. In addition, irregular surface with pits were observed in Group 4 ST72'. [Figure 2]g. In [Figure 2]h, we can observe a irregular surface morphology with pits and voids of Group 5-ST24. For the concentration ratio of 1:4 and 1:6, 24 hours duration was insufficient to form a homogeneous nanofilm of TiO2. [Figure 3]a, shows roughest surface morphology of Group 6-TT, that is, uncoated TMA wire. [Figure 3]b and [Figure 3]c represents the SEM images of Group 7-TT48 and Group 7-TT72. We can observe a smoother surface morphology of TMA wire coated with 1:2 ratio. [Figure 3]d, [Figure 3]e, [Figure 3]f, reveals the SEM images of Group 10TT24, Group 10TT48, and Group 11TT48. All these groups showed better surface morphology with a relatively smoother surface. [Figure 4]c and [Figure 4]d suggest that at the least concentration ratio (1:8), even 48 hours and 72 hours of dipping duration was insufficient to form a homogenous covering. Rather we can observe increased crystallization and peeling of TiO2 layer on SS wire. At highest concentration (1:2), 24 hours of dipping duration is insufficient to form a homogeneous nanofilm of TiO2 over TMA archwires. The surface morphology was rough with voids and uncoated areas [Figure 4]e, [Figure 4]f. On an average, groups of concentrations (1:2, 1:4, and1:6) except 1:8 showed better surface characteristics [Figure 4]a, [Figure 4]b, [Figure 4]c, [Figure 4]d, [Figure 4]e, [Figure 4]f. Among these three concentrations, all the groups with 48 hours of dipping duration exhibited good surface characteristics. Group 4-ST48 has the least frictional resistance in both dry and wet conditions among all the groups of SS wire while in TMA, Group 9-TT48 has the least frictional resistance in both conditions [Table 3]. Intragroup comparison between Group 2-ST48 and Group 4-ST48 among SS wires was not significant (p = 1.000) in both dry and wet conditions. Rest all other intragroup comparison of SS wires have significant difference among each other (p = 0.001) in both dry and wet conditions. Intragroup comparison among TMA wires showed that there was no significant difference between Group 7-TT48 and Group 8-TT48 (p = 1.000) in both dry and wet conditions and also there was no significant difference between Group 7-TT48 and Group 9-TT48 (p = 1.000) and between Group 8-TT48 and Group 9-TT48 (p = 1.000) only in wet condition. But during dry condition both of the above intragroup comparison showed significant difference (p = 0.002 and 0.001). Rest all other intragroup comparison of TMA wires showed significant difference (p = 0.001) [Table 4]. Intergroup comparison between SS and TMA showed that there was significant difference among all the groups (p = 0.001) except Group 2-ST48 and Group 7-TT48 (p = 0.481-dry and 1.000-wet) in both the conditions [Table 5].
|Figure 1: XRD pattern of the colloidal solution with the concentration ratio of 1:6. (Solid blue diamond represents rutile phase and solid red circle represents anatase phase)|
Click here to view
|Figure 2: Scanning Electron Microscopic images of uncoated and TiO2 coated SS archwires. (a) SEM image of Group 1-ST (uncoated SS wire), (b) SEM image of Group 2-ST24, (c) SEM image of Group 2-ST48, (d) SEM image of Group 2-ST72, (e) SEM image of Group 3-ST72, (f) SEM image of Group 4-ST48, (g) SEM image of Group 4-ST72, (h) SEM image of Group 5-ST24|
Click here to view
|Figure 3: Scanning electron microscopic images of uncoated and TiO2-coated TMA archwires (a) SEM image of Group 6-TT (uncoated TMA wire), (b) SEM image of Group 7-TT48, (c) SEM image of Group 7-TT72, (d) SEM image of Group 8-TT24, (e) SEM image of Group 8-TT48, (f) SEM image of Group 9-TT48|
Click here to view
|Figure 4: Scanning electron microscopic images of poor coating of TiO2 on SS and TMA archwires (a) SEM image of Group 3-ST24, (b) SEM image of Group 4-ST24, (c) SEM image of Group 5-ST48 (red arrow indicates pealing of TiO2 coating), (d) SEM image of Group 5-ST72 (blue arrow indicates crystallization of TiO2 nanoparticles and red arrow indicates uncoated bare wire surface), (e) SEM image of Group 7-TT24, (f) SEM image of Group 9-TT24|
Click here to view
|Table 4: Statistical analysis of intra-group comparison between SS wires and TMA wires|
Click here to view
|Table 5: Statistical analysis of inter-group comparison between SS and TMA wires|
Click here to view
| Discussion|| |
Resistance during tooth movement may occur due to physical or biological factors. Use of nanoparticles in various studies has led to the development of many orthodontic wires with improved frictional characteristics.,,, The antibacterial effect of TiO2-coated wires has been evaluated without considering frictional properties., Various physical and chemical approaches have been used to prepare TiO2 thin films, including sol-gel and pulsed laser deposition. Hosseingholi et al. synthesized nanocrystalline TiO2 sols through the hydrolysis of tetra-isopropyl orthotitanate at different pH values and room temperature. We used the Sol-gel method, which is the most facile and cost-effective route that not only omits the requirement of high temperatures, toxic chemicals, and expensive equipment but also offers several advantages such as the better homogeneity of the structure, high purity of starting materials, and possibility to control the porosity and structure of a fixed, three-dimensional network of gels with better coating stability. The ratio of 1:1 (1 part of TiO2 and 1 part of deionized water) was not observed in the colloidal state and thus discarded. XRD findings indicated the presence of an equal size of TiO2 nanoparticles among different concentrations. Approximately 83% of the nanocrystalline structure of TiO2 was in the anatase phase, as indicated by Hosseingholi et al. In contrast to the findings of our study, a previous study reported that the rutile phase exerts a greater effect on improvement in surface characteristics. However, another study indicated that both the anatase and rutile phases of TiO2 can improve surface characteristics equally. With a decrease in the TiO2 concentration, the duration required to form a smooth and uniform nanofilm increased. Moreover, at a ratio of 1:8, crystallization and peeling of TiO2 nanoparticles were observed. The 24-hours dipping duration was insufficient to form a uniform TiO2 nanofilm. Only a higher ratio (1:2) and 72-hours dipping duration led to the peeling of the TiO2 nanofilm surface, as observed through SEM. All the coated wires of SS and TMA exhibited a significantly decreased frictional coefficient compared with their respective uncoated controls (p = 0.001). Intergroup comparison indicated that most of the SS wire groups demonstrated significantly decreased friction compared with TMA wire groups except in a few groups (Group 2-ST48 and Group 7-TT48). TMA wires contain 70% titanium, which makes their surface rougher than that of SS wires, resulting in an increase in friction. This finding is in accordance with those of previous studies., At a higher concentration (1:2), TMA required 48 hours of dipping to form a smoother TiO2 nanofilm with uniform deposition. TiO2-coated SS/TMA wires under wet conditions consistently exhibited the lowest frictional resistance values. This finding is supported by a study using fullerene-like nanoparticles. SS/TMA coated archwires with a ratio of 1:6 and a dipping duration of 48 hours demonstrated better results with respect to both surface characteristics and frictional resistance compared with other ratios (1:2 and 1:4). Lower concentrations of TiO2 (<1:6) did not produce promising results. A dipping duration of 48 hours was optimal because <48 hours led to irregular coating and >48 hours led to the crystallization and peeling of the nanofilm layer. Keerthi et al. suggested that the smoothness of TiO2-coated wires was lost at the end of 1 month of intraoral use. Improper concentration and coating time of TiO2 may be responsible for the loss of coating. The variation in results may be due to the intraoral environment (in-vivo) in the previous study which is not the exact replica of our in-vitro experimental condition, although we used both dry and wet conditions.
| Conclusion|| |
Optimal concentration and coating time required for surface modification are elaborated in detail and concluded that:
- The optimum concentration of TiO2 ranges from 1:2 to 1:6 with a dipping duration of 48 hours.
- Increasing or reducing the TiO2 concentration did not affect the nanoparticle size of TiO2.
- Frictional forces decreased in almost all the coated wires of SS and TMA except in some cases with a dipping duration of <48 hours.
- Saliva could reduce friction in both the TiO2-coated wires (SS and TMA).
- TMA wire relatively required increased dipping durations even at higher concentrations.
Financial support and sponsorship
Conflicts of interest
There are no conflicts of interest.
| References|| |
Kusy RP, Whitley JQ. Friction between different wire bracket configurations and materials. Semin Orthod 1997;3:166-77.
Kusy RP, Whitley JQ, Mayhew MJ, Buckthal JE. Surface roughness of orthodontic archwires via laser spectroscopy. Angle Orthod 1988;58:33-45.
Kang T, Huang SY, Huang JJ, Li QH, Diao DF, Duan YZ. The effects of diamond like carbon films on fretting wear behaviour of orthodontic archwire-bracket contacts. J Nanosci Nanotechnol 2015;15:4641-7.
Mezeg U, Primožic J. Influence of long-term in vivo
exposure, debris accumulation and archwire material on friction force among different types of brackets and archwires couples. Eur J Orthod 2017;39:673-9.
Zhang H, Guo S, Wang D, Zhou T, Wang L, Ma J. Effects of nanostructured, diamondlike, carbon coating and nitrocarburizing on the frictional properties and biocompatibility of orthodontic stainless-steel wires. Angle Orthod 2016;86:782-8.
Anuradha P, Varma NK, Balakrishnan A. Reliability performance of titanium sputter coated Ni–Ti arch wires: Mechanical performance and nickel release evaluation. Biomed Mater Eng 2015;26:67-77.
Cao S, Liu B, Fan L, Yue Z, Liu B, Cao B. Highly antibacterial activity of N-doped TiO2 thin films coated on stainless steel brackets under visible light irradiation. Appl Surf Sci 2014;309:119-27.
Ghasemi T, Arash V, Rabiee SM, Rajabnia R, Pourzare A, Rakhshan V. Antimicrobial effect, frictional resistance, and surface roughness of stainless-steel orthodontic brackets coated with nanofilms of silver and titanium oxide: A preliminary study. Microsc Res Tech 2017;80:599-607.
Liu JX, Yang DZ, Shi F, Cai YJ. Sol–gel deposited TiO2 film on NiTi surgical alloy for biocompatibility improvement. Thin Solid Films 2003;429:225-30.
Tidy DC. Frictional forces in fixed appliances. Am J Orthod Dentofacial Orthop 1989;96:249-54.
Vincenzo D, Rongo R, Ametranoa G, Spagnuoloa G, Manzoa P, Martina R, et al
. Evaluation of surface roughness of orthodontic wires by means of atomic force microscopy. Angle Orthod 2012;82:922-8.
Kusy RP, Whitley JQ, Gurgel AJ. Comparisons of surface roughness and sliding resistances of 6 titanium-based or TMA-type archwires. Am J Orthod Dentofacial Orthop 2004;126:589-603.
McQuillin B, Ray AK, Turner ML, Seddon AB. Photoelectric characteristics of lead phthalocyanine/titanium oxide structures. J Phys D Appl Phys 2000;33:2683-6.
Garzella C, Comini E, Tempesti E, Frigeri C, Sberveglieri G. Synthesis of nanostructured and nanoporous TiO2-AgO mixed oxide derived from a particulate Sol-Gel route: Physical and sensing characteristics. Sens Actuators B 2000;68:189-96.
Hosseingholi M, Pazouki A, Hosseinnia SH, Aboutalebi J. Room temperature synthesis of nanocrystalline anatase sols and preparation of uniform nanostructured TiO2 thin films: Optical and structural properties. Phys D Appl Phys 2011;44:05540.
Bessekhouad Y, Robert D, Weber JV. Preparation of TiO2 nanoparticles by Sol-Gel route. Int J Photoenergy 2003;5:153-8.
Caratto V, Aliakbarian B, Casazz AA, Setti L, Bernini C, Perego P, et al
. Inactivation of Escherichia coli on anatase and rutile nanoparticles using UV and fluorescent light. Mater Res Bull 2013;48:2095-101.
Baby RD, Subramaniam S, Arumugam I, Padmanabhan S. Assessment of antibacterial and cytotoxic effects of orthodontic stainless-steel brackets coated with different phases of titanium oxide: An in-vitro study. Am J Orthod Dentofacial Orthop 2017;151:678-84.
Muguruma T, Iijima M, Brantley WA, Mizoguchi I. Effects of a diamond-like carbon coating on the frictional properties of orthodontic wires. Angle Orthod 2011;81:141-8.
Anto DV, Rongo R, Ametranoa G, Spagnuoloa G, Manzoa P, Martinac R, et al
. Evaluation of surface roughness of orthodontic wires by means of atomic force microscopy. Angle Orthod 2012;82:132-5.
Katz A, Redlich M, Rapoport L, Wagner H, Tenne R. Self-lubricating coatings containing fullerene-like WS2
nanoparticles for orthodontic wires and other possible medical applications. Tribol Lett 2006;21:135-9.
Venkatesan K, Kailasam V, Sridevi Padmanabhan S. Evaluation of titanium dioxide coating on surface roughness of nickel-titanium archwires and its influence on Streptococcus mutans adhesion and enamel mineralization: A prospective clinical study. Am J Orthod Dentofacial Orthop 2020;158:199-208.
[Figure 1], [Figure 2], [Figure 3], [Figure 4]
[Table 1], [Table 2], [Table 3], [Table 4], [Table 5]